This is an accelerated laboratory corrosion test method that can be used to determine the corrosion resistance of automotive assemblies and components. It is cyclic in nature, i.e.; test specimens are exposed to changing climates over time.
Test specimens are placed in an enclosed chamber and exposed to a changing climate that comprises of the following 3 part repeating cycle. 4.0 hours exposure to a continuous indirect spray of neutral (pH 6.5 to 7.2) salt water solution, which falls-out on to the specimens at a rate of 1.0 to 2.0ml/80cm²/hour, in a chamber temperature of +35C . This is followed by 2.0 hours of air drying in a climate of 20 to 30%RH at +60C. This is followed by 2.0 hours exposure to a condensing water climate (wetting) of 95 to 100%RH at +50C. The number of cycle repeats and therefore the test duration is variable.
The maximum transition times between each part of the test cycle are also specified as follows:
From salt spraying to air drying within 30 minutes.
From air drying to wetting within 15 minutes.
From wetting to salt spraying within 30 minutes.
Necessary cookies are absolutely essential for the website to function properly. This category only includes cookies that ensures basic functionalities and security features of the website. These cookies do not store any personal information.
Any cookies that may not be particularly necessary for the website to function and is used specifically to collect user personal data via analytics, ads, other embedded contents are termed as non-necessary cookies. It is mandatory to procure user consent prior to running these cookies on your website.